United States Department of Agriculture
Strength andStiffness of Light-FrameSloped Trusses Ronald W.
Wolfe Donald H. Percival Russell C. Moody
Bending tests conducted on 42 wood trusses provided information
on the effects of truss slope and lumber modulus of elasticity
(MOE) on truss strength and stiffness. Two 28-foot-span Fink truss
configurations with slopes of 3/12 and 6/12 were tested. Component
lumber was all No. 2 grade southern pine separated into low,
medium, and high MOE categories. All trusses exhibited linear load
vs. deformation behavior up to and beyond twice their design load
range. Variations in load carrying capacity were small within a
slope/stiffness category, and lumber stiffness appeared to be
closely correlated with load capacity, failure mode, and truss
stiffness. Information in this report is an important first step
toward formulating improved structural analysis procedures for roof
Keywords: Roof, Trusses, Light-frame, Strength, Stiffness, Test,
Wolfe, Ronald W.; Percival, Donald H.; Moody, Russell C.
Strength and stiffness of light-frame sloped trusses. Res. Pap. FPL
471. Madison, WI: U.S. Department of Agriculture, Forest Service,
Forest Products Laboratory; 1986. 16 p.
A limited number of free copies of this publication are
available to the public from the Forest Products Laboratory, One
Gifford Pinchot Drive, Madison, WI 53705-2398. Laboratory
publications are sent to over 1,000 libraries in the United States
The Laboratory is maintained in cooperation with the University
PageIntroduction . . . . . . . . . . . . . . . . . . . . . . . .
Literature Review . . . . . . . . . . . . . . . . . . . .
Objectives and Scope . . . . . . . . . . . . . . . . . . . . . .
. . . . . .
Research Methods . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . .Truss Design . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . .Material . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . .Truss Fabrication . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . .TrussTests . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
.Analysis Methods . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . .
Results . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . .Lumber Properties . . . . . . . . . . . .
. . . . . . . . . . . . . . . . .TrussStiffness . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . .Truss Strength . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Analysis of Results . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . .TrussStiffness . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . .Truss Strength . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . .
Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . .
Literature Cited . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . .
Appendix-Summary of Truss Member MOE Measurements . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . .
3 3 4 4 4 5
6 6 6 7
10 10 11
United States Department of Agriculture
Er ra t a
Strength and Stiffness of Light-Frame Sloped Trusses
Research Paper FPL 471 Errata
In Figure 10, page 12. the uni t of measure for the ver t ical
axis should be
as wri t ten .
"Mil l ion lb / in . 2 should be the unit of measure for the
Wolfe, Ronald, W.; Percival, Donald H.; Moody, Russell C.
Strength and Stiffness of Light-Frame Sloped Trusses. Res. Pap. FPL
471. Madison, WI: U.S. Department of Agriculture. Forest Service,
Forest Products Laboratory; 1986. 16 p.
Strength and Stiffness of Light-FrameSloped Trusses1
Ronald W. Wolfe,* Research General Engineer Donald H.
Percival,** Research Professor of Wood Technology Russell C.
Moody,* Research General Engineer
*Forest Products Laboratory, Madison, WI **Small Homes Council,
University of Illinois, Champaign, IL
Roof systems used in residential construction have an
outstanding record of structural performance. This is due in part
to the use of conservative design assumptions. Current design
procedures make no attempt to account for this conservatism;
therefore, the inherent margin of safety in these roof systems
cannot be quantified. This report covers the first phase of a
research program to evaluate the relative reliabilities of various
roof system designs. Specifically, the objective of this study is
to characterize the strength and stiffness performance of two
light-frame truss configurations.
Designers of steel and concrete structures have taken the lead
in applying reliability theory to structural design. They have
published standards which improve design efficiency by taking into
account variability of material as well as loads. The trend toward
reliability-based design, evident for these materials, points the
direction for improvements to engineered wood design. Most of the
work required to characterize structural loads has already been
done. The major concern of researchers dealing with
reliability-based design of wood structures, therefore, is to
characterize the probability distributions associated with
Another concept which should receive greater attention is system
design. Current roof design procedures are based on single member
design and give little credit to the advantage of repetitive member
systems. In light-frame trussed roof systems, each truss is
designed as though all its chord and web members have a near
minimum clear wood strength and the maximum allowable strength
reducing characteristic permitted for their grade. In addition, it
is assumed that each truss in the system must be designed to carry
its tributary area of design load. Limited recognition is given to
load sharing mechanisms, either within the truss or between
trusses. In order to improve roof system design, analysis methods
must be developed to minimize unrecognized conservatism and provide
a more accurate assessment of the true margin of safety. Methods
are needed a) to accurately characterize the distribution of truss
stiffness and strength, and b) to predict how loads are distributed
among rafters within a roof system. This report presents individual
truss test results which will be used to evaluate the accuracy of
theoretical models developed to characterize roof system
1This study was conducted in cooperation with the Southern Pine
Inspection Bureau and the Truss Plate Institute.
Industry design standards for metal plate connected trusses were
first presented by the Truss Plate Institute (TPI) in 1960. The
approach was deterministic, connections were assumed to transfer
only axial loads, and chord elements were analyzed as simple beams
with superimposed moments.
Increased popularity of computers in the 1960s resulted in
significant improvements to truss design through the development of
computer programs capable of providing indeterminate analyses. The
most notable of these programs for the truss industry was the
Purdue Plane Structures Analyzer (PPSA) (Suddarth 1972, Suddarth
and Wolfe 1983). PPSA gave a more accurate analysis of member
stresses than the TPI procedure, however, it was considered too
costly to run and too complicated to use for everyday truss design.
PPSA was therefore used by the truss industry as a means of
checking and improving determinate analysis methods described in
TPls design specifications (TPI 1978).
Other truss analysis programs have also been developed for the
analysis of wood structures. A program called SADT, developed by
Foschi (1977a & b), provides options to account for sheathing
contributions and plastic behavior in truss plate connectors. This
program permits characterization of displacement behavior beyond
the design range whereas PPSA is a design tool, oriented to the
analysis of trusses and frames within the elastic range.
The truss industry design methods have evolved following methods
recommended in the National Design Specification for Wood
Construction (NDS), (Nat. For. Prod. Assoc. 1982). The NDS
recommends use of lumber stress values derived according to
standards published by the American Society for Testing and
Materials (ASTM) Standard D 245 (ASTM 1983c). These values are
based on a clear wood strength (ASTM D2555-83), which is estimated
to be at the 5th percentile of the distribution of all clear wood
pieces. Strength reductions for grade characteristics assume knots
and/or slope of grain are the maximum permitted. Thus each truss is
designed as though each member is of minimum strength and quality
for its species and grade.
Egerup (1975, 1979, undated) used Monte Carlo simulation, along
with programs similar to those developed by Suddarth and Foschi, to
assess the distribution of stiffness and load capacity of roof
trusses. Results of his studies suggest that the 5th percentile
value for truss load carrying capacity is greater than the load
capacity predicted using the 5th percentile value for strength of
individual members. He attributes this to several factors:
(a) loads are distributed away from weak members (b) there is a
low probability that a member with the
5th percentile strength will be located at the point of maximum
(c) two or more members may show some form of plastic
deformation before a truss actually fails.
Along with the development of computer models, data have also
been collected on loads, member strength properties, and truss
connector plate moment and axial load resistance. Thurmond et al.
(1983) provided a summary of roof loads and derivation of
distribution parameters. Truss lumber strength and stiffness
properties have been collected (Gerhards and Percival 1979) and
characterized (Hoyle et al. 1979) to indicate correlations between
stiffness and strength. The In-grade test program being conducted
as a cooperative effort between lumber grading agencies and the
Forest Products Laboratory (FPL) is supplying full-size member
strength and stiffness data for bending, tension and compression
(Galligan et al 1980).
A number of studies have been conducted to characterize the
load-slip behavior of several truss connector plates (Foschi 1979;
Perkins et al. 1962; Quaile and Keenan 1979). Also, work conducted
by Zahn (1982, 1984) at FPL, and by Buchanan at the University of
British Columbia (Buchanan 1984) on the analysis of the effects of
combined axial-bending loads provide a data base for the analysis
of astress limit state for the chord and web members. Necessary
material property information either is or soon will be available
to begin development of a reliability-based design procedure for
roof systems. Before these design procedures can be implemented,
however, available material properties, analysis models, and load
information must be refined and decisions must be made regarding
limit state criteria.
Objectives and Scope Research Methods
The objective of this study is to characterize the strength and
stiffness performance of two light-frame truss configurations.
Results will be used in the development and evaluation of a truss
strength/stiffness model. Undamaged trusses from this study will
also be used in a subsequent study to evaluate the influence of
system interactions on the load-deflection response of trusses used
in a full-scale roof.
Forty-two full-size trusses were evaluated. Twenty-four were
tested to failure and the other 18 were tested to 1.25 times their
design load to determine their stiffness characteristics.
The two truss configurations considered were designed by
representatives of the TPI. Prior to manufacturing the trusses, the
lumber was sorted into three modulus of elasticity (MOE)
categories. For each combination of truss configuration and MOE
category, seven trusses were manufactured using metal plate
connectors; three trusses were tested to 1.25 x design load and
four trusses were tested to failure. A description of the truss
test variables is given in table 1.
The truss configurations were selected to be typical of commonly
used residential roof trusses. Both designs were for 28-foot-span
Fink trusses to be spaced 24 inches on center. Both were designed
for top chord load only. The 3/12 sloped truss (fig. 1) had a
design live load of 17.5 Ib/ft2,and the 6/12 sloped truss had a
design live load of 23 Ib/ft2.The dead load was 10 Ib/ft2 in each
case. Total design loads for the 3/12 trusses (1,540 pounds), and
for the 6/12 trusses (1,850 pounds), were for 10 years duration and
were controlled by stresses in the top chord. The ratio of actual
stress to allowable stress (sec. 303.6 of TPI 1978) at some
location in the top chord of each truss design was equal to 1.0.
The bottom chord had no vertical load, thus the ratio of actual to
allowable was much lower (0.46 for the 3/12 and 0.20 for the
In both cases, the metal plates were designed to be larger than
normal (i.e. either thicker or larger area) to force failure to
occur in the wood. The rationale for this over plating was that the
allowable stresses for lumber include an adjustment for load
duration and those for steel do not. A short-term test to determine
truss strength would have agreater chance of resulting in metal
failure than wood failure, if both were selected on the basis of
the same ratio of imposed stress to allowable stress at the design
load. Industry cooperators recommended that it was important to
force failure to occur in the wood in order to supply data to
evaluate the ability of a computer model to predict the probability
of wood failure.
Table 1 .Description of southern pine truss tests
Number of trusses
MOE 3/12 Slope 6/12 Slope Totalcategory Loaded to Loaded to
Loaded to Loaded to1.25 x DL1 failure 1.25 x DL
Low (L) 3 4 3 4 14Medium (M) 3 4 3 4 14High (H) 3 4 3 4 14
TOTAL 9 12 9 12 421 DL = design load.
Figure 1.Test trusses with 3/12 and 6/12 top chord slopes were
designed for this study. In all cases, the heel and bottom chord
splice joints were made using 16-gauge metal connector plates.
Remaining plates were 20 gauge. Plate dimensions (in inches) are
shown near each joint. (ML85 5612)
The southern pine lumber used for this study was No. 2 2 x 4 in
lengths of 12, 14, and 16 feet. Each piece was visually graded to
meet the requirements for No. 2 and marked with an identification
number. It was then passed through a Continuous Lumber Tester (CLT)
machine to measure an average MOE value along its length.
Additional evaluations of the lumber are discussed in Appendix A.
Part of the lumber, obtained from Alabama, had MOE values ranging
from 1.4 to 2.6 million lb/in2. A second portion, obtained from
Arkansas, had MOE values ranging from 0.8 to 1.4 million
A 16-gauge metal truss plate supplied by one manufacturer was
used at the heel and bottom chord splice joints, and a 20-gauge
plate by another manufacturer was used at all other joints. In both
cases, the teeth were approximately 3/8-in. long by 1/8-in. wide
(3/8 in. by 5/32 in. for the 16 gauge, and 5/16 in. by 1/8 in. for
the 20 gauge, see fig. 2).
The lumber was divided into three MOE categories according to
the average MOE values determined by the CLT machine. Lumber in the
low stiffness (L) category had MOE values ranging from 0.8 to 1.4
million lb/in2. The range for the medium stiffness (M) was 1.4 to
2.0 million lb/in2,and for the high stiffness (H) was 2.0 to 2.6
million lb/in.2.The few pieces with MOE values outside of these
ranges were not used.
Figure 2.Truss plates used in the fabrication of the test
trusses. The 16-gauge steel plate (top) had a tooth density of
and the 20-gauge steel plate (bottom) had a tooth density of 8
teeth/in.2. In both cases, the individual teeth are approximately
3/8-inch long by 1/8-inch wide. (ML85 5613)
Various lengths were randomly selected within each of the three
MOE categories and assigned to 1 of 14 trusses (7 with 3/12 slope
and 7 with 6/12 slope). Lumber for each truss was marked with a
four part identification which gave the slope of the truss (3,6),
its MOE category (L,M,H), a sequence number (1-7), and a code
related to the location in the truss (fig. 3). Hydraulic presses
were used to install the truss plates during manufacture. The
trusses were then delivered to the testing laboratory where they
were stored inside for at least 7 days prior to testing.
The trusses were evaluated in a horizontal position using atest
facility that consisted of parallel reaction brackets laid into a
concrete floor (fig. 4). Hydraulic loading rams, lateral restraint
braces, and reaction pads were attached to these brackets and could
be moved in one direction in the plane of the floor to accommodate
any truss configuration with a span of up to 35 feet and a height
of up to 10 feet.
The ends of the truss were placed on 4-inch-wide reaction pads
spaced 28 feet apart (outside to outside). Thus, the span from
center-to-center of each reaction was 27 feet 8 inches.
Twenty-eight concentrated loads were applied at 12-inch intervals
along the top chord of each truss to simulate a uniform load
application. These loads were applied using 14 hydraulic cylinders
spaced 24 inches apart. Each cylinder was centered on a distributor
beam which transferred the load to the top chord through two load
points spaced 1 foot apart.
Deflection readings were taken using a taut wire stretched
between points on the centroidal axis of the bottom chord above the
reactions. Wood lath strips extending from seven points along the
top chord held mirrored gauges under the wire to enable measurement
of top chord deflections. Mirrored gauges were also placed at five
points along the bottom chord. These positions are shown as the
circled locations numbered 1-12 on figure 3.
Calibrated proving rings positioned at the reactions were used
to measure the relationship between the hydraulic pump pressure
gauge and the applied load on the truss. Two pilot trusses of each
slope were tested to develop pressure versus load curves for the
two truss configurations. These calibration procedures were also
checked using electronic load cells. Measurements taken from the
pressure versus load curves were found to be within 2 percent of
those measured directly using the load cells. For the majority of
tests, end grain Douglas-fir blocks were inserted at the reaction
points and loads were read from the pressure gauge.
An initial load of 1,000 pounds was applied to each truss and
held for 5 minutes to check for alignment, settlement, final
adjustment, and then removed. Loads were then applied in increments
of 0.25 x design load, and deflection readings were taken at each
load increment after the load had been maintained for 5 minutes.
Total time of test varied from about 1/2 hour for those tested to
determine stiffness only to nearly 2 hours for the stronger trusses
tested to failure.
For each combination of top chord slope and MOE category, three
trusses were loaded to 1.25 x design load and four trusses were
loaded to failure. For the trusses loaded to failure, deflection
readings were taken at each increment until either failure appeared
imminent or four times design load was reached. Ultimate load and
failure locations were recorded for each truss along with comments
regarding apparent influencing factors and failure progression.
Data obtained included lumber stiffness, and the stiffness,
strength, and failure mode of each truss. Linear regression
analyses were used to show how lumber MOE, truss slope, and load
level affected truss response to increased load. Evaluations of the
effect of lumber MOE on truss strength and failure mode were
conducted to aid the prediction of truss failure. By correlating
lumber and truss stiffness to
Figure 3.Identification of truss members and deflection points.
Truss members are identified by use and location: top chord (TC),
bottom chord (SC), and web (WB). Member numbers are assigned left
to right corresponding to the orientation of the truss in the test
apparatus. Deflection points are circles and are also numbered left
to right. (ML85 5614)
Figure 4.Truss test facility at the Small Homes Council,
University of Illinois, Champaign-Urbana with a 6/12 truss. (M85
strength and failure mode of those trusses tested to
destruction, it was possible to estimate the load capacity of those
trusses tested to only 1.25 x design. This information will be used
in the planning stages of full-scale roof tests which will use the
nondestructively tested trusses.
Individual trusses will be referred to by their three-part Table
2.Summary of modulus of elasticity values for lumber identification
code number, as discussed previously under in each truss category
truss fabrication. Truss members have an additional code 3/12 Slope
6/12 Slope related to their location in the truss (fig. 3).
category Average Coefficient Average CoefficientMOE
of ofIn all cases, the discussion of truss stiffness in the load
MOE variation MOE variationrange from 0 to 1.25 x design load
Million lb/in.2 Pct Million lb/in.2 Pcton all seven trusses in
each slope-MOE category. Discussion of truss strength, however,
refers only to the four Low (L) 1.23 9.4 1.24 9.2 trusses in each
category which were tested to failure. Medium (M) 1.67 9.1 1.73
High (H) 2.30 6.7 2.31 7.2Lumber Properties
Table 2 gives a summary of MOE values measured for lumber used
in the trusses in each slope/stiffness category. MOE values for
each truss member are given in the Appendix.
Moisture content readings (resistance meter) taken at the time
of testing indicated that all members of each truss had close to
the same moisture content. Trusses 6H1 through 6H5 had moisture
contents of 9 percent. All other trusses were at 10 percent.
Within the range of design load, deflections appeared to be
symmetric and linear with load. Figure 5 shows typical deflection
profiles for a truss loaded to 1, 2, and 3 times design load. A
parabolic curve connecting the panel point deflections is
indicative of the global deflection of the truss, while deviations
from this curve represent localized bending deflections in the
loaded top chord. Significant localized bending deflection is
evident in the top chord while all points on the bottom chord
appeared to fit the expected parabolic pattern.
Figure 5.Deflection profile of a low stiffness 3/12 sloped truss
(3L7) loaded to 1, 2, and 3 times the design load of 1,540 lb.
Loads were applied at l-foot intervals along the top chord, and
deflections were measured at all web connections and midway between
web connections for both top and bottom chords. (ML85 5615)
Figure 6 is a typical set of load versus deflection curves for
one side of a symmetric truss. Deflections of node points 3, 4, and
6 represent global deflection of the truss. Deflections measured at
mid-panel points (1 and 5) are a combination of localized bending
of the top chord and global deflection of the truss.
Due to its close proximity to the heel reaction, the global
deflection of point 1 is much smaller than that for point 5. In
fact, for every truss, point 5 (or its symmetric point 6) in the
panel adjacent to the peak deflected more than any other point
measured. If the node point deflections are used as an indicator of
truss stiffness, figure 6 indicates that a linear load deflection
model would be an adequate predictor of truss global deflections up
to twice design load.
Table 3 provides a summary of ultimate loads, and gives failure
for each truss tested to destruction. These trusses failed during
the 5-minute holding period between load applications. Of the 24
trusses tested to failure, 17 had lumber failures in the top chord,
3 failed due to knots or brash wood in the tension chord, and 4
failed at web connections. Examples of all types of failures are
shown in figure 7.
The 17 top chord failures included 12 associated with knots, and
5 in wood free of knots. All these failures were due to combined
bending and compression stresses. Failures in knot-free wood
included three which were initiated over the compression web
connection and two unusual failures. Truss 3M3 failed when a piece
of wood flew out of the end panel of the top chord (fig. 8 top).
Inspection of the break in truss 3M3 suggested that some ring shake
may have been present in a region of two edge knots. When
compressive load on the remaining effective section exceeded the
threshold required to cause it to buckle, it suddenly pushed a
2-foot-long piece away from the surface. The other unusual failure
occurred in truss 6M1. The top chord member (TC1) seemed to fail in
horizontal shear (fig. 8 bottom). Lengthwise splits in the area of
the neutral axis of this member ran from the web connection to the
splice joint between members TC1 and TC2.
Figure 6.Typical plot of truss deflection versus the design load
ratio. Points 3, 4, and 6 correspond to web-chord connections.
Point 1 is mid-panel of the top chord section adjacent to the truss
heel and point 5 is mid-panel adjacent to the peak. (ML85 5616)
Table 3.Ultimate load and description of failure
Truss Failedidentification Ultimate load
Design load member1ratio Description of failure
3/12 SLOPED TRUSSES
3L1 4,620 3.00 TC13L3 5,000 3.25 TC13L5 4,240 2.75 TC43L7 5,000
Average 4,720 3.06
3M1 6,540 4.25 BC13M3 5,780 3.75 TC43M5 6,540 4.25 TC13M7 7,320
Average 6,550 4.25
3H2 7,320 4.75 WB23H4 8,080 5.25 WB2, WB3 3H6 7,320 4.75 BC13H7
7,320 4.75 TC1
Average 7,510 4.88
6/12 SLOPED TRUSSES
6L2 6,010 3.25 TC16L3 6,010 3.25 TC16L5 6,470 3.50 TC26L7 6,010
Average 6,120 3.31
6M1 10,630 5.75 TC16M2 9,240 5.00 TC26M4 9,240 5.00 TC26M7 9,240
Average 9,590 5.19
6H1 11,090 6.00 WB3
6H2 7,390 4.00 WB3
6H6 8,780 4.75 TC1
6H7 9,240 5.00 TC4
Average 9,120 4.94
Edge knot Edge knots Edge knot Brash failure at edge of heel
Centerline knot Shake and edge knots Edge knots Splinter in
Peak plate connection Peak plate connection Edge knot Centerline
Brash failure over web connection Edge knot Edge knot Brash
failure over web connection
Shear at top chord splice Edge knot Centerline knot Splinter
over web connection
Wood failure in web bottom chord connection Wood failure in web
bottom chord connection Centerline knot over web connec- tion
Centerline knot over web connec- tion
Primary piece of lumber in the truss (fig. 3) involved in
Figure 7.Examples of different failure types. Top: Top chord
failures resulting from combined bending and compressive stresses.
chord failures resulting from tensile stresses. Bottom:
Connection failures in a bottom chord joint (left) and a peak joint
(right). (M85 0003)
Analysis of Results
Figure 8.Unusual failures showing a buckling type failure (top)
and shear type failure (bottom) in top chord. (M85 0004)
The three tension chord failures occurred in the 3/12 slope
trusses. Two of these were associated with knots, and one occurred
in brash wood close to the heel joint (middle of fig. 7).
All four connection failures were in the high MOE trusses-two in
each slope category (bottom of fig. 7). For the 3/12 trusses these
failures occurred at the web-to-peak joint. In these cases, the
peak plates were misplaced by as much as 5/8 inch resulting in
reductions in the number of teeth connecting the plate to the web.
Estimated reduction in plate holding capacity was 13 percent for
truss 3H2 and 29 percent for 3H4. For the two 6/12 trusses it was
the bottom chord-tension web connection that failed. In both these
cases, a layer of wood as thick as the tooth length was torn out of
the web member.
Table 2 gives the mean values and coefficient of variation of
MOE values for the lumber in each truss category. There was little
difference between the MOE of lumber used in the 3/12 and 6/12
Table 4 gives three values of the average global stiffness for
trusses in each slope-MOE category. These values were derived by
using a linear regression analysis to determine the slope of the
load versus deflection curve of each truss up to a load of 1.25
times the design load. Within each category, these slopes were
averaged for the top chord node points (3 and 10), the bottom chord
node points (4 and 9), and the peaks (6) (fig. 3). For 3/12
trusses, it is evident that deflection increases slightly as you
move toward the center of the truss. However, this is not the case
for the 6/12 trusses. For these trusses, the average peak
deflections were about the same as those of the top chord (nodes 3
Table 4.Truss stiffness represented by the average slope of the
load deflection curves determined at the five web-to-chord
MOE Top chord2 Bottom chord3 Peak4
category Average COV5 Average COV5 Average COVs
Lb/in. Pct Lb/in. Pct Lb/in. Pct
Low 3,460 8.8 3,270 9.1 3,220 9.6Medium 5,030 6.9 4,570 6.2
4,670 8.4High 6,020 5.3 5,600 6.5 5,550 6.6
Low 9,820 6.3 9,040 5.1 9,740 3.5M e d i u m 1 3 , 9 2 0 9.7
13,010 7.0 14,540 6.8High 18,690 9.4 17,820 8.0 18,740 9.11Values
are based on averages of seven tests up to 1.25 times design
2Averages of points 3 and 10 shown in fig. 3.
3Averages of points 4 and 9 shown in fig. 3.
4Point 6 shown in fig. 3.
5Coefficient of variation.
The effects of lumber MOE on truss stiffness can be Table
B.-Linear regression parameters for deflection of 3/12 evaluated by
comparing values given in tables 2 and 4. sloped trusses. Values
correspond to average web-chord Table 2 shows that the average
lumber MOE increased connection deflections at three increments of
about 40 percent with each change in lumber MOE category (DL);
(L-M and M-H). Table 4 shows that the 6/12 trusses exhibit
DEFLECTION = A (Design Load Ratio) + B
about a 40 percent stiffness increase for both steps in Load
increment lumber MOE category. For the 3/12 trusses, the low to
Truss 0 - D L D L - 2 x D L 2 x D L - 3 x D L medium step is also
close to 40 percent: however, the No. medium to high step is closer
to 20 percent. This reduction A B A B A B
in stiffness increment may be due to the higher member 3L1 0.454
-0.002 0.487 -0.036 1.004 -1.070 stresses that develop in the low
sloped, high MOE lumber 3L3 0.471 0.007 0.545 -0.067 0.850 -0.677
trusses. These higher member stresses in turn place greater stress
on the truss plate connections which may have caused significant
slip in the truss joints. This slip could
cause these trusses to have less apparent stiffness. Table 4also
shows that the 6/12 trusses were about three times as
stiff as the 3/12 trusses. 3M5 0.292 0.001 0.308 -0.017 0.466
-0.3323M7 0.330 0.000 0.345 -0.008 0.437 -0.191
Linear regression techniques were also used to characterize
Average 0.318 0.000 0.345 -0.026 0.483 -0.303the load deflection
response of trusses beyond the design load. This analysis, which
was based only on those trusses 3H2 0.262 0.004 0.229 0.038 0.349
-0.203tested to failure, resulted in a trilinear curve to represent
the 3H4 0.247 0.000 0.344 -0.097 0.303 -0.016
average performance of trusses in each category. Slopes 3H6
0.289 -0.002 0.293 -0.005 0.390 -0.2003H7 0.271 0.003 0.259 0.015
were derived for three segments of a load vs. deflection Average
0.267 0.000 0.282 -0.015 0.349 -0.148curve which represents the
average deflection measured at five truss node points (Points 3, 4,
6, 9, and 10, fig. 3). These segments were selected as multiples of
design load (DL) beginning at zero and ending at 3 times design
load. Table 6.Linear regression parameters for deflection of 6/12
Tables 5 and 6 give the parameters derived to fit straight sloped
trusses. Values correspond to average web-chord line segments to
these load intervals. These parameters connection deflections at
three increments of design load were averaged for each stiffness
category to give the (DL); trilinear curves shown in figure 9.
These regression DEFLECTION = A (Design Load Ratio) + B
parameters were derived to model deflection as a function of
Load increment the design load ratio (applied load/design load). In
order to Truss 0 - D L D L - 2 x D L 2 x D L - 3 x D L convert the
slope (A) of the first segment (zero to design No. load) shown in
tables 5 and 6 to a truss stiffness, one must A B A B A B
multiply the truss design load by 1/A. 6L2 0.178 -0.006 0.191
-0.019 0.222 -0.0826L3 0.183 -0.003 0.242 -0.061 0.345 -0.268
Truss Strength 6L56L7
Lumber MOE had an effect on both the failure modes and Average
0.186 0.000 0.239 -0.053 0.335 -0.245
strength of the trusses. Most of the low and medium MOE trusses
failed due to bending in the end panels of the top
chord which would be expected based on the truss design. 6M4
0.123 -0.002 0.137 -0.016 0.138 -0.018For the high MOE trusses,
there was a mixed mode of 6M7 0.121 -0.004 0.170 -0.053 0.149
-0.010failure with half of them failing in the web-to-chord Average
0.124 0.000 0.142 -0.018 0.127 0.012connection.
6H1 0.110 -0.003 0.119 -0.013 0.112 0.002
The effect of lumber MOE on strength is shown in figure 10 which
contains plots of the maximum load of each truss
6H7 0.109 -0.002 0.116 -0.009 0.106 0.012versus the average MOE
of its component lumber. Within Average 0.102 0.000 0.114 -0.012
0.115 -0.015most MOE-slope categories, the trusses show little
strength variation. An exception is the high MOE 6/12 trusses. The
highest and lowest strength trusses in this group were the first
two tested, and some difficulties in setup and calibration of the
equipment may have influenced the failure loads. Also, the two
types of failures (both bending-compression and web-to-chord
connection) may have contributed to the higher variability for this
Figure 9.Trilinear curves fit to load-deflection data of three
MOE categories of 3/12 sloped trusses (left) and 6/12 sloped
trusses (right). Parameters for these curves are given in tables 5
Figure 10.Ultimate load of trusses as affected by the average
MOE of truss members. Quadratic regression and 95 percent
confidence limits were derived on the basis of 12 trusses tested to
failure for the 3/12 slope. (ML85 5618)
A regression analysis was used to determine the relationship
between lumber MOE and truss strength. The regression lines shown
in figure 10 for the 3/12 trusses includes the mean and both the
upper and lower 95 percent confidence limits on the prediction
curve for individual values.
A quadratic model gave a significantly better fit than either
alinear or logarithmic model for the 3/12 trusses:
P = 7953 MOE - 1522 MOE2 - 2650
whereP = maximum load (Ibs)
MOE = average lumber modulus of elasticity (million
For the 3/12 trusses, 91 percent of the variation in strength
could be explained by the model.
A satisfactory regression relationship could not be obtained for
the 6/12 trusses; mainly due to the high MOE trusses which had both
high variability and lower-than-expected strength. Possible reasons
for this have been previously discussed and this group was omitted
from further analysis. Because the failure modes of the trusses in
both slope categories with both low and medium MOE were similar,
the expected performance of the 6/12 trusses was represented as a
constant multiple of the 3/12 trusses.
The plot shown for the 6/12 trusses in figure 10 is the function
used for the 3/12 trusses multiplied by 1.38 which is the average
ratio of strength of the low and medium MOE ranges of 6/12 and 3/12
trusses. The fit of this curve suggests that the 6/12 trusses with
low and medium MOE lumber may have been slightly more sensitive to
the lumber MOE than the 3/12 trusses. For the small amount of data
involved, however, the 38 percent increase on the 3/12 model gives
a reasonable fit to the 6/12 data.
Conclusions Literature Cited
These test results demonstrate truss performance characteristics
which will be useful in modeling the stiffness and strength of
light-frame wood trusses to be used in tests to evaluate a
full-scale roof system model. Specifically:
1. All trusses tested showed linear deflection performance up to
twice the design load and only slight deviations from linearity up
to three times design.
2. Test results show little variability in truss strength and
stiffness within a given slope-MOE category.
3. There appears to be a definite correlation between lumber
stiffness, load capacity, and failure mode for these trusses.
Caution should be used in applying these results to production
1. All contained larger truss plates than required in order to
force failure to occur in the wood member.
2. No loads were applied directly to the bottom chord as would
be expected in most construction.
American Society for Testing and Materials. StandardMethod for
Establishing Structural Grades and Related Allowable Properties for
Visually Graded Lumber. ASTM D245-81. Philadelphia, PA: American
Society for Testing and Materials; 1983.
American Society for Testing and Materials. StandardMethods for
Establishing Clear Wood Strength Values. ASTM D2555-81.
Philadelphia, PA: American Society for Testing and Materials;
Buchanan, A. H. Strength model and design methods for bending
and axial load interaction in timber members. Vancouver, BC:
University of British Columbia, Department of Civil Engineering;
1984. Ph. D. thesis.
Egerup, A. R. Monte Carlo simulation of the ultimate load of
timber trusses. Structural Research Laboratory, Technical
University of Denmark; undated.
Egerup, A. R. Theoretical and experimental determination of
stiffness and ultimate load of timber trusses. Rep. R62. Structural
Research Laboratory, Technical University of Denmark; 1975.
Egerup, A. R. European practice and future development in the
design of metal plate connected wood trusses. In: Proceedings,
Metal plate wood truss conference; Forest Products Research
Society; 1979: 117-122.
Foschi, R. O. Analysis of wood diaphragms and trusses. Part I:
Diaphragms. Canadian Journal of Civil Engineering. 4(3): 345-352;
Foschi, R. O. Analysis of wood diaphragms and trusses. Part II:
Truss plate connections. Canadian Journal of Civil Engineering.
4(3): 353-362; 1977b.
Foschi, R. O. Truss plate modeling in the analysis of trusses.
in: Proceedings, Metal plate wood truss conference; Forest Products
Research Society; 1979: 1557-1574.
Galligan, W. L.; Green, D. W.; Gromala, D. S.;Haskell, J. H.
Evaluation of lumber properties in the United States and their
application to structural research. Forest Products Journal.
30(16): 45-51; 1980.
Gerhards, C. C.; Percival, D. H. Species grades and mechanical
properties of lumber sampled from truss fabricators. In:
Proceedings, Metal plate wood truss conference; Forest Products
Research Society; 1979. pp. 21-31.
Hoyle, R. J.; Haskell, J. H.; Galligan, W. L. Characterizing
lumber properties for truss research. In: Proceedings, Metal plate
wood truss conference; Forest Products Research Society; 1979. pp.
National Forest Products Association. National design
specification for wood construction. NFPA, 1619 Massachusetts
Avenue, Washington, DC; 1982.
Perkins, R. H.; Suddarth, S. K.; Dale, A. C. Rotational
resistance of three-membered nailed joints subjected to bending
moment. Purdue University Research Bulletin No. 753, Lafayette, IN.
Quaile, A. T.; Keenan, F. J. Truss plate testing in Canada: Test
procedures and factors affecting strength properties. In:
Proceedings, Metal plate wood truss conference; Forest Products
Research Society; 1979: 105-112.
Suddarth, S. K. A computerized wood engineering system: Purdue
plane structures analyzer. Res. Pap. FPL 168. Madison, WI: U.S.
Department of Agriculture, Forest Service, Forest Products
Suddarth, S. K.; Wolfe, R. W. Purdue plane structures analyzer
IIA computerized wood engineering system. Gen. Tech. Rep. FPL-40.
Madison, WI: U.S. Department of Agriculture, Forest Service, Forest
Products Laboratory; 1983.
Thurmond, B. M.; Woeste, F. E.; Green D. W. Roofloads for
reliability analysis of lumber properties data. Wood and Fiber
Science. 16(2): 278-297; 1983.
Truss Plate Institute. Design specification for metal plate
connected wood trusses. TPI 78. 1978 TPI, 583 DOnofrio Drive, Suite
200, Madison, WI 53719.
Truss Plate institute. Design specification for metal plate
connected parallel chord wood trusses. PCT 80, 1980 TPI, 583
DOnofrio Drive, Suite 200, Madison, WI 53719.
Zahn, J. J. Strength of lumber under combined bending and
compression. Res. Pap. FPL 391. Madison, WI: U.S. Department of
Agriculture, Forest Service, Forest Products Laboratory; 1982.
Zahn, J. J. Strength of southern pine 2 x 4 beam columns. NTIS
ADA 143-138; 1984.
Appendix Summary of Truss Member MOE Measurements
Two different values of MOE were obtained from the CLT machine
for each piece of lumber. One was the average value which is an
average of many short span values measured along the length. The
other is called the low point which is the minimum value measured
along the length. More details on span length and method of
measuring are available from the equipment manufacturer.1
Prior to truss fabrication, a third value was measured for each
piece using a flatwise bending test having a center point load on a
12-foot simple span. In the main text of this report, only the CLT
average values were used. Tables Al and A2 give these values for
each 3/12 and 6/12 truss member respectively.
Table A3 compares all three values of MOE for each of the MOE
categories. This table includes more lumber than was used in
manufacturing the trusses, thus the data may not agree with table
Low point CLT values were about 3/4 of the average CLT values.
For the high MOE lumber, the flatwise and CLT average values were
quite close. But, for both the low and medium MOE lumber, the
flatwise bending MOE was slightly less than the CLT average.
1lrvington-Moore, P.O. Box 23038, Portland, OR 97223.
Table A1 .Modulus of elasticity for each truss member of the
3/12 trusses. These values were determined using a CLT
Truss TC1 TC2 TC3 TC4 BC1 BC2 WB1 WB2 WB3 WB4No.
LOWE3L1 0.97 1.31 1.33 1.23 1.37 1.26 1.09 1.21 1.23 1.09 3L2
1.30 1.23 1.32 1.26 1.31 1.25 1.32 1.14 1.14 1.11 3L3 1.06 1.03
1.29 1.34 1.17 1.11 1.32 1.34 1.39 1.32 3L4 0.96 1.33 1.39 1.27
1.01 1.35 1.11 1.37 1.34 1.09 3L5 1.24 1.24 1.29 0.97 1.39 1.19
1.29 1.03 1.24 1.11 3L6 1.13 1.32 1.37 1.33 1.23 1.34 1.32 1.25
1.25 1.11 3L7 1.37 1.33 1.33 1.13 1.33 1.15 1.09 1.31 1.21 1.28
MEDIUM E 3M1 1.76 1.69 1.72 1.85 1.55 1.79 1.83 1.89 1.57 1.83
3M2 1.63 1.56 1.89 1.47 1.49 1.41 1.58 1.58 1.58 1.58 3M3 1.60 1.65
1.72 1.87 1.80 1.63 1.52 1.85 1.52 1.52 3M4 1.55 1.74 1.74 1.87
1.59 1.49 1.55 1.54 1.61 1.55 3M5 1.77 1.65 1.69 1.60 1.75 1.93
1.55 1.89 1.90 1.55 3M6 1.46 1.75 1.29 1.42 1.91 1.92 1.52 1.57
1.52 1.52 3M7 1.71 1.56 1.90 1.74 1.81 1.81 1.75 1.54 1.85 1.88
Table A2.Modulus of elasticity for each truss member of the 6/12
trusses. These values were determined using a CLT machine.
Truss TC1 TC2 TC3 TC4 BC1 BC2 WB1 WB2 WB3 WB4No.
6L1 1.27 1.26 1.24 1.08 1.29 1.08 1.14 1.35 1.26 1.40 6L2 1.03
1.24 1.38 1.31 1.23 1.28 1.14 1.34 1.00 1.17 6L3 1.18 1.17 1.38
1.16 1.31 0.98 1.17 1.25 1.36 1.34 6L4 1.30 1.19 1.16 1.21 1.28
1.17 1.28 1.39 1.05 1.34 6L5 1.31 1.26 1.28 1.24 1.11 1.37 1.02
1.40 1.06 1.346L6 1.18 1.30 1.30 1.19 1.23 1.12 1.02 1.39 1.36 1.28
6L7 1.09 1.17 1.19 1.30 1.37 1.38 1.34 1.30 1.05 1.40
6M1 1.96 1.87 1.79 1.94 1.97 1.71 1.66 1.50 1.70 1.45 6M2 1.92
1.79 1.87 1.89 1.74 1.41 1.61 1.66 1.87 1.62 6M3 1.94 1.58 1.46
1.99 1.46 1.74 1.87 1.85 1.81 1.81 6M4 1.87 1.64 1.43 1.93 1.98
1.63 1.93 1.61 1.59 1.68 6M5 1.95 1.46 1.46 1.91 1.91 1.59 1.80
1.68 1.93 1.97 6M6 1.93 1.43 1.46 1.98 1.91 1.74 1.70 1.97 1.62
1.85 6M7 1.95 1.43 1.64 1.96 1.54 1.61 1.50 1.60 1.45 1.59
HIGH E 6H1 2.14 2.37 2.37 2.38 2.41 2.45 2.25 2.25 2.36 2.36 6H2
2.09 2.18 2.18 2.52 2.31 2.21 2.46 2.36 2.58 2.36 6H3 2.38 2.23
2.23 2.03 2.28 2.07 2.45 2.42 2.46 2.39 6H4 2.07 2.47 2.47 2.05
2.35 2.15 2.42 2.39 2.45 2.48 6H5 2.07 2.04 2.58 2.57 2.50 2.14
2.58 2.58 2.48 2.58 6H6 2.28 2.35 2.19 2.29 2.07 2.02 2.18 2.03
2.39 2.50 6H7 2.32 2.35 2.19 2.10 2.07 2.20 2.18 2.06 2.44 2.50
3H1 2.36 2.44 2.54 2.31 2.32 2.25 2.44 2.45 2.50 2.03 3H2 2.40
2.32 2.46 2.41 2.27 2.27 2.18 2.47 2.51 2.44 3H3 2.44 2.32 2.34
2.39 2.25 2.33 2.50 2.45 2.36 2.44 3H4 2.36 2.46 2.34 2.25 2.25
1.81 2.06 2.47 2.36 2.44 3H5 2.26 2.44 2.54 2.34 2.34 2.28 2.44
2.51 2.50 2.39 3H6 2.07 2.04 2.04 2.13 2.02 2.05 2.24 2.15 2.31
2.24 3H7 2.15 2.25 2.25 2.08 2.09 2.07 2.24 2.15 2.31 2.24
Table A3.Comparison of measured MOE values for lumber used in
the fabrication of the test trusses. CLT values were measured in
the mill and flatwise bending values were measured just prior to
MOE ApproximateContinuous lumber tester (CLT)
Flatwise bendingnumber of Average Low-point STDSTD Mean COV2 ERR
category specimens1 Mean COV2 STD Mean COV2 ERR3ERR 3
Million Million Million Million Million Millionlb/in. 2 Pct
lb/in. 2 lb/in. 2 Pct lb/in. 2 lb/in. 2 Pct lb/in. 2
Low 165 1.25 9.5 0.009 (4) (4) (4) 1.12 12 0.02Medium 150 1.74
10.6 0.015 1.26 16.3 0.017 1.65 14.3 0.019High 120 2.29 6.9 0.014
1.72 11.9 0.019 2.27 9.8 0.011Sample size for various methods of
MOE measurement may vary by 3.
2Coefficient of Variation for sample.
3Standard error of the estimate of mean value.
4Data not obtained on a significant part of the sample.